| ||Format||Pages||Price|| |
|8||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$62.00||  ADD TO CART|
This specification establishes the requirements for electrodeposited zinc coatings applied to iron or steel articles for corrosion protection purposes. Electrodeposited zinc-coated steel wires or sheets are not covered here. The coatings shall be provided in four standard thickness classes in the as-plated condition or with one of three types of supplementary finishes. The surfaces of the articles shall under go pre-plating basis metal cleaning, pre- and post-coating treatment for reducing the risk of hydrogen embrittlement, and reactivation and supplementary treatments. Coatings should be sampled, prepared, tested and conform accordingly to specified requirements as to appearance (luster and workmanship), thickness, adhesion, corrosion resistance, and hydrogen embrittlement.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers material and process requirements for electrodeposited zinc coatings applied to iron or steel articles to protect them from corrosion.
1.2 This specification is not intended to provide the design activity with all the background needed to properly specify their zinc coating requirements. The users of Specification B633 are encouraged to review this specification in its entirety including the appendices, and access the supplementary papers, other standards, and published literature referenced herein and within other related references.
1.3 The coatings are provided in four standard thickness classes ( ), in the as-plated condition or with one of five types of supplementary finishes ( ).
1.4 High strength metals, including high strength steels having a tensile strength greater than 1700 MPa (247 ksi, 46 HRC) should not be zinc electroplated in accordance with this specification.
1.5 It does not cover continuous processes for electrodeposited zinc coated steel wire or sheets (see Specification for sheets).
1.6 For zinc electroplating of mechanical fasteners, the purchaser is encouraged to consider Specification .
1.7 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.8 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.9 This standard has been revised to address RoHS requirements that seek to limit the exposure of workers and the public from exposure to toxic metals. Additional types V and VI have been added to permit non-chromate passivate treatments to be used in replacement of hexavalent chromium.
1.10 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A591/A591M Specification for Steel Sheet, Electrolytic Zinc-Coated, for Light Coating Weight [Mass] Applications
B117 Practice for Operating Salt Spray (Fog) Apparatus
B183 Practice for Preparation of Low-Carbon Steel for Electroplating
B201 Practice for Testing Chromate Coatings on Zinc and Cadmium Surfaces
B242 Guide for Preparation of High-Carbon Steel for Electroplating
B254 Practice for Preparation of and Electroplating on Stainless Steel
B320 Practice for Preparation of Iron Castings for Electroplating
B322 Guide for Cleaning Metals Prior to Electroplating
B374 Terminology Relating to Electroplating
B487 Test Method for Measurement of Metal and Oxide Coating Thickness by Microscopical Examination of Cross Section
B499 Test Method for Measurement of Coating Thicknesses by the Magnetic Method: Nonmagnetic Coatings on Magnetic Basis Metals
B504 Test Method for Measurement of Thickness of Metallic Coatings by the Coulometric Method
B567 Test Method for Measurement of Coating Thickness by the Beta Backscatter Method
B568 Test Method for Measurement of Coating Thickness by X-Ray Spectrometry
B571 Practice for Qualitative Adhesion Testing of Metallic Coatings
B602 Test Method for Attribute Sampling of Metallic and Inorganic Coatings
B697 Guide for Selection of Sampling Plans for Inspection of Electrodeposited Metallic and Inorganic Coatings
B748 Test Method for Measurement of Thickness of Metallic Coatings by Measurement of Cross Section with a Scanning Electron Microscope
B762 Test Method of Variables Sampling of Metallic and Inorganic Coatings
B849 Specification for Pre-Treatments of Iron or Steel for Reducing Risk of Hydrogen Embrittlement
B850 Guide for Post-Coating Treatments of Steel for Reducing the Risk of Hydrogen Embrittlement
D2092 Guide for Preparation of Zinc-Coated (Galvanized) Steel Surfaces for Painting
F1470 Practice for Fastener Sampling for Specified Mechanical Properties and Performance Inspection
F1940 Test Method for Process Control Verification to Prevent Hydrogen Embrittlement in Plated or Coated Fasteners
F2078 Terminology Relating to Hydrogen Embrittlement Testing
ISO StandardISO/TR 20491
ICS Number Code 25.220.40 (Metallic coatings)
UNSPSC Code 11101704(Steel)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM B633-19, Standard Specification for Electrodeposited Coatings of Zinc on Iron and Steel, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top